Download presentation

Presentation is loading. Please wait.

1
**Example 5.2: Anhydrous Sodium carbonate **

Structure with strong harmonic modulation of positions and ADP. Chemical formula: Na2CO3 3d incommensurate commensurate Alpha 9.02, 5.21, , 90, 90 P63/mmm Beta 8.98, 5.25, , 90.33, 90 C2/m Gamma 8.92, 5.25, , , 90 C2/m(0) q=(0.182,0,0.322) Delta 8.90, 5.24, , , 90 C2/m(0) q=(1/6,0,1/3) 757K 628K 170K Change of rotation symmetry Change of translation symmetry Gamma Delta Alpha Beta The main change of the structure occurs during the alpha beta transition which changes rotation symmetry. Although modulations in gamma and delta phase are very strong they only modify the beta structure keeping the rotation symmetry unchanged.

2
**Data for the phase gamma**

Single crystal data measured with KUMA four-circle diffractometer Input files: naco.hkl, naco.cif_od Frame scaling, absorption correction: done with software of diffractometer Unit cell: a=8.9338, b=5.2678, c=6.0565, α= β= , γ= q vector: (0.1776, 0, ) c* a*

3
Import wizard 1 2 3

4
Symmetry wizard 1 2

5
3 Data processing was done with C centering.

6
**4 5 6 Space group from main reflections**

Superspace group from satellite reflections Symbol C2/m(0b0)s0 means: 3d symmetry C2/c q vector (0 β 0) shift by ½ in x4 M50: symmetry x1 x2 x3 x4 symmetry -x1 x2 -x3 -x4+1/2 symmetry -x1 -x2 -x3 -x4 symmetry x1 -x2 x3 x4+1/2 6

7
**Structure solution wizard**

The only reason for the random seed is compatibility with the text of Jana Cookbook. Convergence with R~21%

8
**Output of Superflip confirms the symmetry**

9
**The initial structure model**

1 2 3

10
Individual atoms

11
File M40

12
Structure plots or

13
**The plot helps to identify oxygens**

C1 and C2 will be changed to oxygens with “Edit atoms” tool of Jana

14
**Structure refinement Refinement of the initial structure model**

Adding position modulation waves

15
**Refinement with harmonic ADP and four position modulation waves for all atoms**

16
**Fourier maps and Contour plots**

Coordinates of Na1: x,y,z Sections to plot: x2-x4 Range of x2: from (y – 2Å/b) to (y + 2Å/b) step 0.02Å Range of x4: from 0 to 2, step 0.02 Stacking of sections: x2-x4 x3(1) x1(1) x2-x4 x3(2) x1(1) …. x2-x4 x3(n) x1(1) x2-x4 x3(1) x1(2) x2-x4 x3(2) x1(2) x2-x4 x3(n) x1(m) Range of x1: from (x-1Å/a) to (x+1Å/a) Range of x3: from (z-1Å/c) to (z+1Å/c) Fourier maps and Contour plots

17
**Observed and difference Fourier map for Na1 indicates modulation of ADP**

Similar features can be seen in difference maps of other atoms except carbon

18
**Adding ADP modulation waves**

Final refinement Atom Position waves ADP waves Na1 4 3 Na2 2 Na3 O1 O2 C1

19
Final difference maps Contour step 0.1

20
**Interpretation of structure model using Grapht**

Internal coordinate t t=0 t=1

21
**Interpretation of structure model using Dist**

22
**Interpretation of structure model using plots**

Similar presentations

Presentation is loading. Please wait....

OK

A Brief Description of the Crystallographic Experiment

A Brief Description of the Crystallographic Experiment

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on center of gravity Ppt on inhabiting other planets outside the solar Ppt on natural and artificial satellites orbiting Ppt on omission of articles Ppt on ocean food web Ppt on national education policy 1986 calendar Ppt on mobile and wireless networks Ppt on service marketing 7 p's Ppt on articles of association of a company Ppt on obesity prevention